
data_a

_diffrn_radiation_probe  x-ray
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_pd_spec_mount_mode reflection
_pd_meas_scan_method step
 loop_
_diffrn_radiation_wavelength
_diffrn_radiation_wavelength_wt
 1.5406    1.0000
 1.5443    0.5000
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_diffrn_radiation_monochromator none

_chemical_name_mineral
;
;

_symmetry_space_group_name_H-M P-421m

_symmetry_cell_setting tetragonal
_symmetry_space_group_name_hall 
;
P -4 2ab
;

_cell_length_a  7.75948(23)
_cell_length_b  7.75948(23)
_cell_length_c  5.16799(20)
_cell_angle_alpha 90
_cell_angle_beta  90
_cell_angle_gamma 90
_cell_volume 311.162(22)
_chemical_formula_moiety
;
Al4 Ce0.02 Li0.02 O14 Si2, 4(Sr0.50), 1.96(Ca)
;
_chemical_formula_sum
;
Al4 Ca1.96 Ce0.02 Li0.02 O14 Si2 Sr2
;

_chemical_formula_weight  644.84
_cell_formula_units_Z 1
_exptl_crystal_density_diffrn  3.441145

_exptl_absorpt_coefficient_mu  24.405

_cell_measurement_temperature  300
_diffrn_ambient_temperature  300


_pd_char_colour
;
colourless
;

_pd_proc_number_of_points 5500
_pd_meas_2theta_range_min 10
_pd_meas_2theta_range_max 120
_pd_meas_2theta_range_inc 0.02

_pd_proc_ls_profile_function PearsonVII
_pd_proc_ls_pref_orient_corr
;
no preferred orientation
;

_refine_ls_shift/su_max  0.01000
_refine_ls_R_I_factor 1.78
_pd_proc_ls_prof_wR_factor 9.006
_pd_proc_ls_prof_R_factor 6.935
_pd_proc_ls_prof_wR_expected 7.402
_refine_ls_goodness_of_fit_all 1.217
loop_
_symmetry_equiv_pos_as_xyz
	'x, y, z'
	'-x, -y, z'
	'-x+1/2, y+1/2, -z'
	'-y, x, -z'
	'-y+1/2, -x+1/2, z'
	'y, -x, -z'
	'y+1/2, x+1/2, z'
	'x+1/2, -y+1/2, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Ca Ca 0.33886(19) 0.16114(19) 0.50962(61) 0.49 0.829(72)
Sr Sr 0.33886(19) 0.16114(19) 0.50962(61) 0.5 0.829(72)
Ce Ce 0.33886(19) 0.16114(19) 0.50962(61) 0.005 0.829(72)
Li Li 0.33886(19) 0.16114(19) 0.50962(61) 0.005 0.829(72)
Al1 Al 0 0 0 1 0.36(16)
Al2 Al 0.14038(40) 0.35962(40) 0.9631(10) 0.5 0.32(13)
Si Si 0.14038(40) 0.35962(40) 0.9631(10) 0.5 0.32(13)
O1 O 0.5 0 0.1775(30) 1 1.51(17)
O2 O 0.14885(99) 0.35115(99) 0.2793(16) 1 1.51(17)
O3 O 0.08822(86) 0.16775(87) 0.8118(15) 1 1.51(17)

loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
Ca O1 2.464(11)  .
Ca O2 2.4009(81)  .
Ca O2 2.6429(80) 3_546
Ca O3 2.4948(75)  .
Ca O3 2.8751(74) 6_556
Sr O1 2.464(11)  .
Sr O2 2.4009(81)  .
Sr O2 2.6429(80) 3_546
Sr O3 2.4948(75)  .
Sr O3 2.8751(74) 6_556
Ce O1 2.464(11)  .
Ce O2 2.4009(81)  .
Ce O2 2.6429(80) 3_546
Ce O3 2.4948(75)  .
Ce O3 2.8751(74) 6_556
Li O1 2.464(11)  .
Li O2 2.4009(81)  .
Li O2 2.6429(80) 3_546
Li O3 2.4948(75)  .
Li O3 2.8751(74) 6_556
Al1 O3 1.7632(71) 1_554
Al2 O1 1.7032(75) 3_556
Al2 O2 1.6368(97) 1_556
Al2 O3 1.7297(78)  .
Si O1 1.7032(75) 3_556
Si O2 1.6368(97) 1_556
Si O3 1.7297(78)  .

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
O1 Ca O2 106.13(37) 1_555 1_555
O1 Ca O2 78.89(28) 1_555 3_546
O1 Ca O3 147.3(13) 1_555 1_555
O1 Ca O3 59.37(55) 1_555 6_556
O2 Ca O2 141.78(92) 1_555 3_546
O2 Ca O3 79.57(28) 1_555 1_555
O2 Ca O3 80.98(27) 1_555 6_556
O2 Ca O2 76.35(30) 3_546 4_656
O2 Ca O3 77.79(29) 3_546 1_555
O2 Ca O3 116.86(42) 3_546 5_555
O2 Ca O3 69.06(34) 3_546 6_556
O2 Ca O3 129.38(59) 3_546 8_556
O3 Ca O3 64.92(40) 1_555 5_555
O3 Ca O3 90.89(22) 1_555 6_556
O3 Ca O3 151.3(12) 1_555 8_556
O3 Ca O3 106.73(29) 6_556 8_556
O1 Sr O2 106.13(37) 1_555 1_555
O1 Sr O2 78.89(28) 1_555 3_546
O1 Sr O3 147.3(13) 1_555 1_555
O1 Sr O3 59.37(55) 1_555 6_556
O2 Sr O2 141.78(92) 1_555 3_546
O2 Sr O3 79.57(28) 1_555 1_555
O2 Sr O3 80.98(27) 1_555 6_556
O2 Sr O2 76.35(30) 3_546 4_656
O2 Sr O3 77.79(29) 3_546 1_555
O2 Sr O3 116.86(42) 3_546 5_555
O2 Sr O3 69.06(34) 3_546 6_556
O2 Sr O3 129.38(59) 3_546 8_556
O3 Sr O3 64.92(40) 1_555 5_555
O3 Sr O3 90.89(22) 1_555 6_556
O3 Sr O3 151.3(12) 1_555 8_556
O3 Sr O3 106.73(29) 6_556 8_556
O1 Ce O2 106.13(37) 1_555 1_555
O1 Ce O2 78.89(28) 1_555 3_546
O1 Ce O3 147.3(13) 1_555 1_555
O1 Ce O3 59.37(55) 1_555 6_556
O2 Ce O2 141.78(92) 1_555 3_546
O2 Ce O3 79.57(28) 1_555 1_555
O2 Ce O3 80.98(27) 1_555 6_556
O2 Ce O2 76.35(30) 3_546 4_656
O2 Ce O3 77.79(29) 3_546 1_555
O2 Ce O3 116.86(42) 3_546 5_555
O2 Ce O3 69.06(34) 3_546 6_556
O2 Ce O3 129.38(59) 3_546 8_556
O3 Ce O3 64.92(40) 1_555 5_555
O3 Ce O3 90.89(22) 1_555 6_556
O3 Ce O3 151.3(12) 1_555 8_556
O3 Ce O3 106.73(29) 6_556 8_556
O1 Li O2 106.13(37) 1_555 1_555
O1 Li O2 78.89(28) 1_555 3_546
O1 Li O3 147.3(13) 1_555 1_555
O1 Li O3 59.37(55) 1_555 6_556
O2 Li O2 141.78(92) 1_555 3_546
O2 Li O3 79.57(28) 1_555 1_555
O2 Li O3 80.98(27) 1_555 6_556
O2 Li O2 76.35(30) 3_546 4_656
O2 Li O3 77.79(29) 3_546 1_555
O2 Li O3 116.86(42) 3_546 5_555
O2 Li O3 69.06(34) 3_546 6_556
O2 Li O3 129.38(59) 3_546 8_556
O3 Li O3 64.92(40) 1_555 5_555
O3 Li O3 90.89(22) 1_555 6_556
O3 Li O3 151.3(12) 1_555 8_556
O3 Li O3 106.73(29) 6_556 8_556
O3 Al1 O3 113.04(43) 1_554 2_554
O3 Al1 O3 107.72(39) 1_554 4_556
O1 Al2 O2 118.51(79) 3_556 1_556
O1 Al2 O3 102.1(40) 3_556 1_555
O2 Al2 O3 115.22(55) 1_556 1_555
O3 Al2 O3 101.45(40) 1_555 5_555
O1 Si O2 118.51(79) 3_556 1_556
O1 Si O3 102.1(40) 3_556 1_555
O2 Si O3 115.22(55) 1_556 1_555
O3 Si O3 101.45(40) 1_555 5_555
